02 962 At N CLASS OF CHEMICAL SENSORS FOR GASES ESCFO ON PI4OTOLUMINESCENCE FROM U)MCONSIU!V-MWISON DEPT OF CHEMISTRY G EYER ET RL 6S8 JUL 87
UNCLLSSFE UIS/OC/TR-7/5 OO 14-85-K-6F 2/12 N.
~~~~~~~ w w
w~ ~ ~ .4 a
OFFICE OF NAVAL RESEARCH
Contract N00014-85-K-0631 i ftt(
R&T Code 4134003 4
Technical Report No. UWIS/DC/TR-87/5
A New Class of Chemical Sensors for Gases Based on Photoluminescence from Semiconductor-Derived Interfaces
Gerald J. Meyer, George C. Lisensky, and Arthur B. Ellis*
Prepared for Publication in
Proceedings of the Electrochemical SocietyAccession For
(volume devoted to chemical sensors)FTIS GRA&I
N University of WisconsinUnannounced 0
Department of Chemistry Justification Madison, Wisconsin 53706
Reproduction in whole or in part is permitted for any purpose of the United States Government
This document has been approved for public release and sale; its distribution is unlimited.
should be addressed 11E 9I8?F-
Alf 2 qC12L
SECURIT CLASSIFICATION OF THIS, PAGE
REPORT DOCUMENTATION PAGE
IM. REPORT SECURITY CLASSIFICATION lb. RESTRICTIVE MARKINGS
2a. SECURITY CLASSIFICATION AUTHORITY 3. DISTRIBUTION /AVAILABIUTY OF REPORT
NA Distribution Unlimited; Approved for
2b. OECLASSIFICATIONIDOWNGRADING SCHEDULE Public Release
4. PERFORMING ORGANIZATION REPORT NUMBER(S) S. MONITORING ORGANIZATION REPORT NUMBER(S)
Ga. NAME OF PERFORMING ORGANIZATION 6b. OFFICE SYMBOL Ia. NAME OF MONITORING ORGANIZATION Chemistry Department (| f kabk)
University of Wisconsin-Madiso NA ON
6c ADORESS (City, State, and ZIP Code) 7b. ADDRESS (Cty, State, and ZIP Code)
1101 University Avenue 800 N. Quincy St.
Madison, WI 53706 Arlington, VA 22217
So. NAME OF FUNDING ISPONSORING lab. OFFICE SYMBOL 9. PROCUREMENT INSTRUMENT IDENTIFICATION NUMBER
ORGANIZATION Of applicable)
JNA Contract N00014-85-K-0631 8c ADDRESS (City, State, and ZIP Code) 10. SOURCE OF FUNDING NUMBERS
PROGRAM PROJECT TASK R&T WORK UNIT ELEMENT NO. NO. NO. Code ACCESSION NO
11. TITLE (Include Security Classification)
A New Class of Chemical Sensors for Gases Based on Photoluminescence from Semiconductor- Derived Interfaces
12. PERSONAL AUTHOR(S)
Gerald J. Meyer, George C. Lisensky, and Arthur B. Ellis --
13a. TYPE OF REPORT 13b. TIME COVERED 14. DATE OF REPORT (Year, Month, Day) COUr'C.
Technical FROM TO 4/25/87 11
16. SUPPLEMENTARY NOTATION
Prqpared for publication in Proceedings of the Electrochemical Society (a vo on
17 COSATI CODES I8. SUBJE TE RPAS 1"tintpjars if neesar idlenty ock number) I D GROUP SUB-GROUP n-e ' s gradud-.dSxIr- photluminescence;
dead-layer model; depletion width; surace recombination v lo ty c mical qepsrs ! ydrgen, ammonia, s9 lfur
-\\/ !aloxjla~e, la. and nvar #'n&A & ,,,_11,. !Q
19. AB CT (Continug on reverie if neTVand identify by block number)
The photoluminescence (Z) of semiconductors can be perturbed by exposure of the solid to gases. These physicochemical interactions occurring at the semiconductor surface can be exploited to create a new class of chemical sensors. For homogeneous semiconductors, a dead-layer model has been used to correlate changes in PL intensity with variations in the depletion width W caused by the gas. A graded n- CdTx -"Substrate permits modulation of the PL spectral distribution by gases and is color-code to permit PL changes to be
correlated with variations in the effective electric field present in the solid. Three
structures illustrate these PL effects: Pd-coated semiconductors can respond to hydrogen gas;
semiconductors that have been chemically derivatized with ferrocene can sense volatile oxidants and reductants; and etched semiconductors can respond to sulfur dioxide and
ammonia, presumably through acid-base interactions. All of the structures lend themselves to device fabrication by use of optical fiber technology. t.. .[ t .
20. DISTRIBUTION/AVAILABILITY OF ABSTRACT 21. ABSTRACT SECURITY CLASSIFICATION MUNCLASSIFIEDIUNLIMITED
03SAME AS RPT. 0QOTIC USERS Distribution Unlimited
2a NAME OF RESPONSIBLE INOIVIOUAL 22b. TELEPHONE (Include Area Code) 22c OFFICE SYMBOL
Arthur B. Ellis 608-262-0421
DO FORM 1473,64 MAR 83 APR edition may be used until exhausted SECURITY CLASSIFICATION OF THIS PAGE All other editions are obsolete Unclassified
A NEW CLASS Of CUEMICAL SENSORS FOR GASES BASED ON PEOTOLUmiNESCENCE FaOm SEMICONDUCTOR-DERIVED IrIRFACES Gerald J. Meyer5 , George C. Lisenskyt, and Arthur B. ilLis§
IDepartment of Chemistry, University of 1isconsin-Madison, Madison, Wisconsin 53706
tDepartment of Chemistry, Beloit College Beloit, WisconsiLs -53511
The photoluninescence (PL) of semicqnductors can be perturbed by exposure of the solid to gases. These physicochemical inter- actions occurring at the semiconductor surface can be exploited to create a new class of chemical sensors. For homogeneous semi- conductors, a dead-layer model has been used to correlate changes in PL intensity with variations in the depletion width V caused by the gas. A graded n-CdSxSel-x substrate permits modulation of the PL spectral distribution by gases and is color-coded to permit PL changes to be correlated with variations in the effective electric
field present in the solid. Three structures illustrate these PL effects: Pd-coated semiconductors can respond to hydrogen gas;
semiconductors that have been chemically derivatized with ferrocene can sense volatile oxidants and reductants; and etched semiconduc- tors can respond to sulfur dioxide and &mona, presumably through acid-base interactions. All of the structures lend themselves to device fabrication by use of optical fiber technology.
The intense interest in chemical sesing has prompted a search for new strategies and techniques (1). We have observed that the bulk photoluminescence (PL) of semiconductors can be influenced by chemistry occurring at the surface of the solid, suggesting the use of this effect for chemical sensing (2,3). In this paper we
summarize our past work related to sensing and describe recent results that expand the scope of gas detection.
For homogeneous semiconductors, the PL spectral distribution is essentially unaffected by surface chemistry, and we have employed a dead-layer model (4) to correlate changes in PL intensity with changes in the depletion width W of the solid. The dead-layer model assumes that the region of the semiconductor that supports the
electric field is nonemissive, because electron-hole (e'-h+) pairs
*Address correspondence to this author.
that are formed in that region are separated so rapidly that they are unable to radiatively recombine.
A quantitative expression for the dead-layer model is given in eq. I , and its derivation, based on Beer's Law, is illustrated in Figure 1. In the equation, PL1 and PL2 are the PL intensities for
PL1/FL2 -exp(-G'AD) (1)
the two chemical states of the sensor, wherein the semiconductor is in depletion; a' - (a + "), where a and B are the absorptivities of the semiconductor for the exciting light and emitted light, respect- Lvely; and AD is the change in dead-layer thickness, equated herein with the change in V. An operational test of the dead-layer nodel
involves measuring the PL intensity ratio for several interrogating excitation wavelengths for which the solid has different absorptivities.
A value for AD should be obtained from eq. I that is independent of excitation wavelenSth.
Mettler has shown that a more sophisticated analysis of PL, consisting of plots of PL intensity vs. optical penetration depth, can simultaneously yield the absolute value of V as well as the surface recombination velocity 8, which can also influence PL intensity (5). Implicit in our use of eq. 1 is the notion that S either does not vary between states I and 2 or that it is relatively large (S L/-r and oL2Ii, where L and T are the diffusion length and lifetime of the minority carrier, respectively) (6).
The use of spatially inhomogeneous semiconductors provides a means for modulating the spectral distribution or color of PL. Our
prototypical sample for demonstrating these effects is a graded n-CdSxSel-x substrate. Prepared by the vapor-phase diffusion of S
into single-crystal n-Cdge, the solid's PL is color-coded to identify the spatial origin of e'-h+ pair recombination, since the PL band maximum in CdSgSe .x alloy compositions varies with composition, as shown in eq. 2 (7-10). The depth of these various compositions from
Amax (nm) 718 - 210 X (2)
the surface is determined by Auger electron spectroscopy (AES) with Ar+
sputter etching; typically, the overall thickness of the graded zone is about one micron. The presence of different compositions gives rise to an effective electric field (REP) in these solids, containing contributions from, for example, band-edge and effective-mass gradients.
The affected portion of the PL spectrum identifies, using eq. 2 and the AS data, the depth to which the 317 is altered by chemistry occurring at the surface.
Although PL Is a bulk property, the fact that it is influenced by the presence of an electric field suggested that surface chemistry could affect the emission. Since the depletion width W arises from a mismatch in chemical potentials between the semiconductor and the phase in contact with it, a chemical reaction that strongly affects the
chemical potential of the contacting phase should perturb the PL signal. Alternatively, chemistry that affects the surface recombin- ation velocity S can influence PL.
In sections below we describe three systems that illustrate these concepts. The first two, a semiconductor coated with Pd that senses hydrogen and a derivatized semiconductor that senses volatile oxidants and reductants, have been described and are updated. The third system
is prepared by simple chemical etching and shows strong PL changes when exposed to sulfur dioxide and ammonia gases.
Techniques used for preparing Pd-coated and ferrocene-derivatized samples have been described (2,3,11). Single-crystal c-plates (10 x 10 x I ms) of n-type CdSe were obtained from Cleveland Crystals, Cleve- land, Ohio. The crystals were vapor-grown with resistivities of
"2 ohm-cm. After being cut to dimensions of %0.25 cm2 x 1 m, the samples were etched in Br2/MeOH (1:30 v/v), ultrasonically cleaned in NeOH, and suspended by an edge with DUCO cement from a glass rod. The rod was then placed in an adapter that served as a stopper for a 20-M diameter glass tube that encircled the semiconductor. Two diametric- ally opposed stopcocks near the bottom of the tube and below the semi- conductor served as gas inlets for nitrogen (latheson; 99.99%) and nitrogen mixed with either sulfur dioxide (Matheson; 99.98Z) or amonia (Matheson; 99.99%); a stopcock near the top of the tube and above the semiconductor served as the gas exit and was connected to a flowmeter that was vented into a hood. Experiments were thus done at atmospheric pressure at flow rates of %100 aL/mn. Connections were made with glass tubing and Tygon joints. Sample excitation was accom-
plished with the 457.9 and 514.5 nm lines of a Coherent Radiation CR-12 Ar+ laser and the 632.8 no line:of a Nelles-Griot 10 mW He-Ne laser, using.Corning 2-58 and interference filters. Incident intensities were
typically "l mW/cm2. PL was detected by placing an optical fiber near the emitting surface of the semiconductor and feeding the light into a McPherson 0.3- moanochromstor, equipped with a photon counting detec- tion system. Graded n-CdSxSel-x samples were prepared as previously described (8).
RESULTS AND DISCUSSION
Hydrogen sensint ith palladium-coated semiconductors. When a thin layerof Pd (%100 A) is sputtered onto a single-crystal n-CdS
substrate to form a Schottky barrier, the band edge PL of the substrate lncreases when the ambient gas is changed from V2 to a 31l 32:12
mixture (2). Qualitatively, the enhancement is consistent with a reduction in W in the hydrogen ambient. Quantitatively, the data fit a dead-layer model (eq. 1). A typical enhancement of 70%
corresponded to a reduction in V of nearly 600 X. Connection of electrical leads to the Pd and Cd surfaces produces a Schottky diode whose current-voltage (i-V) properties permit extraction of the
Schottky barrier heights in the two gaseous ambients. Our samples typically exhibited a reduction in barrier height from 0.6 to 0.4 eV in passing from air to hydrogen, the latter value being obtained from both i-V and PL data. Control experiments indicated that the effects observed did not arise from either optical properties of the Pd film or thermal effects. The PL increase could be reversed by exposure to N2 and then to air; ten reproducible cycles of PL changes were obtained in this way.
Color modulation was demonstrated using Pd-coated, graded n-CdSxSel x samples (2). Exposure to 22 caused FL enhancements of up to 501 for wavelengths between 500 and 600 am. The latter wave- length corresponds to PL from an approximately CdS0.5 e0.5 composition, which, from ASS data, lay %0.1 microns from the surface. Thus the 117
in this solid could be altered to roughly this depth.
The origin of these effects has been attributed to a lowering of the Pd work function as a result of the dissolution of hydrogen iv the metal, reducing the Schottky barrier (12). A description of the barrier height reduction in terms of the surface-dipole component of the metal york function has also been proposed (13).
In more recent studies, we were able to sense R2 through similar PL intensity enhancements using n-type, Al-doped ZnSe and Te-doped CdS as substrates; for both of these materials subband gap PL was monitored (11). With CdS as the substrate, we also compared D2 and R2 for PL response. Although the final enhancements for the two gases were the same within experimental error, the D2 response was considerably more sluggish.
Derivatised surfaces as sensors for volatile oxidants and reductants. The covalent bonding of a redox-active film to the surface of a semiconductor provides a second structure for sensing.
Ve thought that the idealized structure sketched below, prepared from an etched n-GaAs surface and a ferrocene derivative (3,14), would yield a change in FL intensity upon oxidation, since the chemi&al potential of the film would be altered. Indeed, exposure of the derivatised surface to gaseous 12 or dry Br2 in a stream of V2 causes the band edge PL intensity of the GaAs substrate to be quenched. The changes fit a dead-layer model, with W increasing by
~~ ~a -, ' ,, .,,, ,"'' ---...- ', 1 •"
E0902 Fe + Fe,
about 250 X upon exposure to 12. That oxidation has taken place was verified by cyclic voltammetry in CR3CI (0.1 8 [nj-u4IjBF4 as supporting electrolyte); this technique also shoved that the film only possessed a few monolayers of redox-active material. Alternatively, oxidation could be verified by using the structure to sense a volatile reductants exposure to gaseous M284 restored the initial n signal. These
spectral changes could be maintained over 10 cycles of alternate exposure to 12 and N2R4.
tn more recent work, we have examined changes in both W and S with film oxidation, using plots of PL intensity vs. optical penetration depth (vide supra) (11). This contactless method of analysis indicates that S is large (%105 cu/s) and unaffected, within experimental error, by fit oxidation with iodine, thus justifying the use of the dead- layer model on this structure.
Other substrates have been employed for observing PL changes (11).
The use of ferrocene-derivatized n-GAs0.6P0 .4 leads to changes.in PL intensity at %650 na that are reversible with N2. And derivatis- ation.of the graded n-CdSxSel-x substrate produces a modest color change, resulting from the quenching of near-surface PL contributions by exposure to 12; these changes, too, are reversible with N2..
A noteworthy observation we have made for these systems is that prolonged exposure to an oxidant may cleave some of the bonds that anchor the redox-active species to the semiconductor: cyclic voltamo- grams of derivatized n-GCas samples obtained after exposure to greater than stoichiometric amounts of 12 vapor reveal a drastically diminished electrochemical signal. While this could restrict solution sensing,
it is less of a concern for gaseous chemical sensing, since in the absence of a solvent even a cleaved redox-active species remains proximate to the surface.
Itched semiconductor surfaces as sensors. The PL from single crystals of n-CdSe that have been etched with Br2/MeOH and exposed to air exhibits a surprising sensitivity to S02 and NH3" Figure 2
reveals that exposure to a flow of pure S02 gas quenches the 720 n PL intensity of CdSe relative to its intensity in N2. The effect Is reasonably reversible, as shown in the figure, but often requires
a "conditioning" period, during which the intensities in N2 and SO2 move considerably from their initial values. Table I shows that the
FL changes fit the dead-layer model: for one garticularly responsive sample, an expansion in W (AD) of about 600 A i observed in passing from R2 to pure S02. It is worth emphasizing that in attributing all of the change in PL to a change in W, we are assuming that S is either
invariant or relatively large in the two gaseous ambients.
In contrast to the SO2 results, exposure to N113 causes a
substantial enhancement in PL intensity relative to the intensity in 52- Figure 3 presents a set of responses to different partial pressures of 313; in each case M2 serves as a carrier gas, yielding a total
pressure of I atm. A squarish response is seen except when pure NH3
is used, when a large transient gives way to a smaller final increase.
The PL data in pure 313 (after the signal stabilized) were found to obey the dead-layer models Table I shows that for one sample H contracted by about 700 A in passing from N2 to N13.
From the data in Figure 3 and analogous experiments for SO2, working response curves can be generated for the two gases, as shown in Figure 4. Although the sensitivity is modest, both gases can be detected at partial pressures of ".10 " atm. Also shown on the figure is the insensitivity of PL to a variety of gases. We found that N2, Ar, CO, C02, R2, and 120 yielded indistinguishable PL signals.
In preliminary experiments, we have seen analogous PL changes with etched, homogeneous CdSxSel._x substrates, indicating that the graded n-CdSxSelx substrates should deliver a change in spectral distribution relative to N2 gas with exposure to NH3 and SO2 gases.
Figure 5 demonstrates this effect for S02 gas: the near-surface PL arising from S-rich compositions is preferentially quenched. Enhance- ment over a comparable spectral region is observed if N33 is
In analyzing these PL changes we were concerned initially with thermal effects. We do not believe that these play a very important role for two reasons. First, at the low incident powers employed
(1 mW/cm2) and with the convective cooling supplied by our substantial gas flow rates ("100 uL/nin), the sample should remain near ambient temperature. Second, there seems to be no correlation between
gaseous thermal conductivities and PL response: the thermal conduct- ivities of N33, CO, and V2 are similar while those of 802 and CO2 are smaller, and that of 82 is an order of magnitude larger (15). We emphasize, too, that in many of our experiments we see substantial PL changes even when only small quantities of SO2 or 313 are mixed into the N2 gas stream.
We believe that the PL changes observed with SO2, a Levis acid, and N33, a Lewis base, and the insensitivity of PL to such molecules
S R2, Ar, 320, CO, and Co2, whose acid-base character is
generally less pronounced, suggest that the observed effects may arise from acid-base interactions. These are "dirty" surfaces. If, for CdSe, we presume the surface to be comprised of Cd, Se, 0, and H atoms,
the opportunities for Lewis acid/base interactions abound. We can envision 802 and NH3 preferring different sites on the surface, resulting in a very different PL response. A greater variety of gas-solid interactions will have to be examined, however, before a
stronger case for this kind of interaction can be made.
The experiments described herein demonstrate that the bulk PL of a semiconductor can be influenced by chemistry occurring at the
surface of the solid, providing a viable mans for sensing certain gases. An actual device can be assembled by using a bifurcated optical fiber: the sensor, placed at the fiber junction, can be irradiated using one leg of the fiber and PL, suitably filtered from the exciting light, detected at the other leg of the fiber.
Although the detection of specific gases has been described, these should be regarded as proof-of-concept experiments. In principle, it should be possible to prepare a semiconductor surface, by etching or coating it, so that a desired species can be detected. There is also no reason in principle why the technique cannot be extended to sensing
Finally, we note the potential of this technique for exploring the steric and electronic landscape of semiconductor-derived interfaces.
This is a contactless, in situ method for probing the terrain of these important interfaces.
This work was generously supported by the Office of Naval Research and the 3M Company. We are grateful to Dr. M.K. Carpenter and Prof. H. Van Ryswyk for their initial studies, which form the basis of this work.
(1) gee, for example, "Solid State Chemical Sensors," J. Janata and R.J. Huber, &ds., Academic Press, New York (1985).
(2) M.K. Carpenter, H. Van Ryswyk, and A.B. Ellis, Langmuir 1, 605 (1985).
(3) II. Van Ryavyk and A. B. Ellis, J. An. Chen. Soc. 108, 2454 (1986.).
(4) R.E. Hollingovorth and J.R. Sites, J. Appl. Phys. 53, 5357 (1982) and references therein.
(5) K. Mettler, Appi. Phys. 12, 75 (1977).
(6) A.A. Burk, Jr., P.B. Johnson, W.S. Robson, and A.S. Ellis, J. Appl. Phys. 59, 1621 (1986).
(7) NH. Streckert, J. Tong, M.K. Carpenter, and A.B. Ellis, J. Electrochen. Soc. 129, 772 (1982).
(8) M.K. Carpenter, N.H. Streckert, and A.B. Ellis, J. Solid State Chen. 45, 51 (1982).
(9) U.H. Streckert and A.B. Ellis, J. Phys. Chen. 86, 4921 (1982).
(10) M.K. Carpenter and A.B. Ellis, J. Electroanal. Chen. 184, 289 (1985).
(11) H. Van Ryawyk, Ph.D. Thesis, University of Wisconsin-Madison (1986).
(12) R. Duo, Surf. Sci. 42, 324 (1973).
(13) D.E. Aapnes and A. Heller, J. Phys. Chen. 87, 4919 (1983).
(14) J.M. Bolts and M.S. Urighton, J. An. Chen. Soc. 101, 6179 (1979).
(15) N.V. Tsederberg, "Thermal Conductivities of Gases and Liquids,"
MIT Press, Cambridge, MA, p. 89 (1965).
Table 1. Dead-Layer Analysis of n-CdSe PL Properties.a Gas a-l, Xb PLgas/PLntrogenc AD, Id
NH3 560 4.1 -730
1500 1.7 -690
SO2 560 0.29 +640
710 0.39 +610
1500 0.64 +580
a. Analysis of changes in band edge PL intensity of an n-CdSe sample that has been etched in Br2/NeOH and exposed to various gases, as described in the Experimental Section.
b. Optical penetration depth of the exciting wavelength, taken as the reciprocal of the absorptivity. Values of a for n-CdSe were taken fron: R.B. Parsons, W. Wardzynski, and A.D. Yoffe, Proc. R. Soc.
London, Ser. A. 262, 120 (1961). The reciprocal absorptivities of 560, 710, and 1500 A correspond to the laser excitation wavelengths 457.9, 514.5, and 632.8 na, respectively.
c. Ratio of PL intensity in the indicated gas to that in nitrogen, both at a pressure of 1 atm.
d. Change in dead-layer thickness in passing from nitrogen to the indicated gas, calculated using eq. 1; an absorptivity of 1.2x 104 cm- 1 (B) was used to correct for self-absorption. Negative values represent a contraction, positive numbers an expansion.
Figure 1. The dead-layer model for analyzing changes in photolumin- escence (PL) intensity for two states, 1 and 2. The symbols CB and VB
represent the solid's conduction and valence band edges, respectively.
For each state, the PL intensity is proportional to the amount of incident light (intensity 10; absorptivity a') absorbed beyond the nonenissive layer whose thickness is D. The ratio of the two PL
intensities leads to eq. 1.
Figure 2. Changes in PL intensity at 720 nm resulting from alternating exposure of an etched n-CdSe sample to N2 (initial response) and SO2. Superimposed on the plot are the original and final PL spectra
obtained in N2 (maxima at 720 nm). Flow rates for both gases were 100 mL/min at 1 acm pressure. The sample was excited using 457.9 nm light.
Figure 3. Changes in PL intensity at 720 nm resulting from alternating exposure of an etched n-CdSe sample to N2 (initial response) and
various partial pressures of NH3 in a N2/NH3 mixed flow. The partial pressures of NH3 are placed beneath the corresponding PL enhancement.
Superimposed on the plot is a PL spectrum obtained in N2 (maximum at 720 nm). Flow rates were 100 nL/mmn at 1 atm total pressure. The sample was excited using 457.9 nm light.
2 1 0
Figure 4. PL response of an etched n-CdSe sample to 502 and NH3 relative to N2 as a function of the partial pressure of the gas in a
N2/S02 or N2/NH3 mixture. Flow rates of 100 mL/ain were used in all experiments. Other gases that gave the same response as N2 are indicated in the figure. The sample was excited using 457.9 nm light.
Figure 5. Changes in PL intensity resulting from exposure of a
graded n-CdSxSel-x sample first to N2 (curve I), then to S02 (curve 2), and finally to N2 again (curve 3). The sample was excited using
457.9 nm light.